Presentation on theme: "Probability of Detection Studies to Quantify Flaw Detection in"— Presentation transcript:
1 Probability of Detection Studies to Quantify Flaw Detection in Composite Laminate StructuresA340 HTP SkinDennis Roach & Tom RiceSandia National LabsFAA Airworthiness Assurance CenterSandia is a multiprogram laboratory operated by Sandia Corporation, a Lockheed Martin Company, for the United States Department of Energy’s National Nuclear Security Administration under contract DE-AC04-94AL85000.
2 Inspection Task Group Team Participants ITG Team Participants CACRC Inspection Task Group Members:Wolfgang Bisle – AirbusChris Dragan – Polish Air Force Institute of TechnologyDon Duncan – US AirwaysJim Hofer – BoeingQuincy Howard – BoeingJeff Kollgaard – BoeingFrancois Landry – Bell HelicopterRobert Luiten – KLM AirlinesAlex Melton – Delta Air AirlinesEric Mitchell – American AirlinesStephen Neidigk – Sandia Labs AANCKeith Phillips – AirbusTom Rice – Sandia Labs AANCDennis Roach – Sandia Labs AANC (Chair)Vilmar da Silva do Vale – EmbraerDennis von Seelen - Lufthansa TechnikDarrell Thornton – UPSSam Tucker – United AirlinesRoy Wong – BombardierRusty Jones, Larry Ilcewicz, Dave Galella, Paul Swindell – FAA
3 Composite Structures on Boeing 787 Aircraft Program Motivation - Extensive/increasing use of composites on commercial aircraft and increasing use of NDI to inspect themComposite Structures on Boeing 787 AircraftCarbon laminateCarbon sandwichFiberglassAluminumAluminum/steel/titanium pylonsComposite Center Wing BoxA380 Pressure BulkheadProgram Goals: Assess & Improve Flaw Detection Performance in Composite Aircraft Structure
4 Sources of Damage in Composite Structure One airline reports 8 composite damage events per aircraft (on avg.) with 87% from impact; cost = $200K/aircraftLightning Strike onThrust ReverserBird StrikeDisbonding at skin-to-honeycomb interfaceTowing Damage
5 Inspection Challenge – Hidden Impact Damage Backside fiber failure from ice impactVisible Impact Damage – external skin fractureBackside Damage – internal skin fracture & core crushExtent of Visible Damage from OutsideDamage from ground vehicleSignificant Internal DamageSource: Carlos Bloom (Lufthansa) & S. Waite (EASA)
6 Composite Honeycomb Flaw Detection Experiment Composite Flaw Detection ExperimentParticipation from over 25 airlines and maintenance depotsIndustry-wide performance curves generated to quantify:How well current inspection techniques are able to reliably find flaws in composite honeycomb structureThe degree of improvements possible through integrating more advanced NDI techniques and procedures.Experiment to Assess Flaw Detection PerformanceBlind application of techniques to study hits, misses, false calls, and flaw sizing
7 737 Composite Horiz. Stabilizer An Experiment to Assess Flaw Detection Performance in Composite Laminate StructuresPurposeDetermine in-service flaw detection capabilities: 1) conventional NDT methods vs. 2) improvements through use of advanced NDT.Optimize laminate inspection procedures.Compare results from hand-held devices with results from scanning systems (focus on A-scan vs. C-scan and human factors issues in large area coverage).Provide additional information on laminate inspections for the “Composite Repair NDT/NDI Handbook” (ARP 5089).A380 Fuselage Section 19737 Composite Horiz. Stabilizer
8 Flaw Detection in Solid Laminate Composites ApproachStatistical design of flaws and other variables affecting NDI - range of types, sizes & depths of flawsStudy factors influencing inspections including composite materials, flaw profiles, substructures, complex shapes, fasteners, secondary bonds, and environmental conditionsPOD and signal-to-noise data gatheringNDI Ref. Stds. prepared to aid experimentExpected Results - evaluate performance attributes1) accuracy & sensitivity (hits, misses, false calls, sizing)2) versatility, portability, complexity, inspection time (human factors)3) produce guideline documents to improve inspections4) introduce advanced NDI where warranted
9 Specimen Design - Flaw Detection in Solid Laminate Composites Specimen Types – Solid laminate carbon (12 to 64 plies)Contoured and tapered surfacesSubstructures – stringers, ribs, spars; honeycomb impedimentBonded & sealed joints; fastenersLarge enough to warrant scanners; complex geometry to challenge scannersCarbon, uniaxial tapeFlaw Types - statistically relevant flaw distribution with range of sizes & depths (near front & back surfaces; in taper regions)1) interply delaminations (“kissing” and air gap)2) substructure damage3) skin-to-stiffener disbonds4) simulated impact damageLow Energy Impact-4590+45
10 Thick Laminate With Complex Taper - Fabrication Flaw templates - ensure proper location of flawsFlawsinserted
11 Thick Laminate With Complex Taper - Fabrication
12 Thick Laminate With Complex Taper Type I Specimen
17 Solid Laminate Flaw Detection Experiment Implementation PODs calculated for overall laminate, by thickness family, by substructure effects, by complex geometry effects, by flaw types, etc inspectors
18 POD Curves for 12-20 Ply Solid Laminate Family Individual and Cumulative ComparisonsFlaw Size (Diameter in Inches)Probability of DetectionOverall:POD[90/95] = 1.29” dia.Constant Thickness(12, 20, 28 plies):POD[90/95] = 0.86” dia.Complex Geometry(tapered, curved, substructure, fasteners, honeycomb):POD[90/95] = 1.49” dia.False Calls: Constant thickness = 0.4/inspectorComplex Geometry = 4.0/inspector34 ft.2 inspection area
19 POD Improvements from Use of Methods to Ensure Proper Coverage Flaw Size (Diameter in Inches)Probability of Detection
20 POD Curves for 20-32 Ply Solid Laminate Family Individual and Cumulative ComparisonsFlaw Size (Diameter in Inches)Probability of DetectionOverall:POD[90/95] = 0.82” dia.Constant Thickness(32 plies):POD[90/95] = 0.74” dia.Complex Geometry(tapered, curved, substructure, fasteners, honeycomb):POD[90/95] = 0.93” dia.Substructure:POD[90/95] = 1.50” dia.False Calls: Constant thickness = 0.8/inspectorComplex Geometry = 0.3/inspector12 ft.2 inspection area
21 Flaw Size (Diameter in Inches) Probability of Detection Desire to Transition Inspectors from “Average” to “Good” to “Outstanding”Flaw Size (Diameter in Inches)Probability of Detection
22 Overall Performance of Pulse-Echo UT for Flaw Detection in Composite LaminatesFlaw Size (Diameter in Inches)Probability of DetectionOverall:POD[90/95] = 1.13” dia.Constant Thickness(32 plies):POD[90/95] = 0.80” dia.Complex Geometry(tapered, curved, substructure, fasteners, honeycomb):POD[90/95] = 1.33” dia.
23 using non-NDI personnel (e.g. A&Ps). Ramp Damage Check Experiment (RDCE) – “Spin Off” Subset of Solid Laminate ExperimentPurpose: to assess new, ultrasonic-based “Go”/“No-Go” equipment that OEM’s plan to deploy at airports and other non-scheduled maintenance depotsusing non-NDI personnel (e.g. A&Ps).Usage Scenario: the equipment will be deployed whenever visual clues or other events occur which warrant closer scrutiny of a composite laminate structure; ground personnel, with appropriate training on such equipment, will set up the equipment in accordance with OEM-supplied procedures, and then make an assessment of the region in question.Limitations: such “Go”/“No-Go” UT equipment is intended to be used to assess local indications or regions only, not for wide-area inspections; equipment operators are directed to very distinct locations.
24 Ramp Damage Check Experiment – Ultrasonic Devices with “Go”/“No-Go” Capabilities General Electric –“Bondtracer”Olympus –“Ramp Damage Checker”
25 Ramp Damage Check Experiment – POD Curves for Composite Laminates Overall:POD[90/95] = 0.78” dia.Similar results for GE Bondtracer and Olympus Ramp Damage CheckerSimilar performance from both inspectors and A&P mechanicsLess spray in individual performancesFlaw Size (Diameter in Inches)Probability of DetectionFalse Calls = 0.6/inspector14 ft.2 inspection area
26 Wide Area and C-Scan Inspection Methods ShearographySAM SystemUltraImage ScannerThermographyMAUSSystemPE Phased Array UTUT Wheel Array
27 Solid Laminate Experiment – Advanced NDI Testing Evaluations Pulsed Thermography – Thermal Wave ImagingPhased Array UT – Olympus OmniscanPhased Array UT – Toshiba Matrix EyePhased Array UT – Sonatest RapidScanPhased Array UT – Boeing MAUS VPhased Array UT – GE RotoArray & PhasorMicrowave – EvisiveDigital Acoustic Video – Imperium AcoustocamUltrasonic Video - DolphiCamLine Infrared – MistrasShearography – LTIShearography – DantecBackscatter X-ray – ScannexAcousto Ultrasonics – Physical Acoustic Corp. T-SCOUTLocked-In Infrared – MovieThermLaser UT – iPhoton
28 Flaw Size (Diameter in Inches) Probability of Detection Sample of POD Results for Composite Flaw Detection Performance of Advanced NDIFlaw Size (Diameter in Inches)Probability of Detection
29 Survey of Industry Composite NDI Training Only 25% of responders currently have special composite NDI training in place
30 Question 15 - If experience level is a factor in determining qualification to perform certain inspections, do you use some sort of apprentice program to expose newer inspectors to such inspections?Question 5 – Do inspectors also receive general composite training to understand composite materials, plies, lay-ups, scarfed repairs, composite design, composite processing, etc.?
31 Conclusions – Inspection of Solid Laminate Structures Results can be used by OEMs and airlines to: 1) define detectability for various flaws/damage, 2) guide NDI deployment & training; used by FAA to produce guidance documents.Flaw Detection - Conventional, manually-deployed PE-UT: POD[90/95] = 1.12” dia.; skin flaw detection is higher, flaw detection in substructure is more challenging (POD[90/95] = 1.34” dia.)False Call rates were extremely low: 1 false call per 17 ft.2 (flaws ≥ 0.25 in.2)Optimum inspection rates = 2 ft.2 /hourNDI Performance Obstacles – attenuation, complex signal reflections, confounding presence of signal harmonics, rapid variations produced by changing/complex geometry, optimum deployment and difficulty with inspecting large areasControlled and Proper Use of Ramp Damage Check “Go”/”No-Go” equipment can produce good performance (POD[90/95] = 0.77” dia.)Caution – proper calibration area must be used; requires good schematics (available?)Cannot be used in taper or changing geometry regions
32 Recommendations – How to move inspections from “average” to “good” to “outstanding” Increased exposure to representative composite inspections – common industry NDI Feedback SpecimensIncreased, focused composite NDI training (ARP covering 1st two bullets)Use of NDI and composite shop apprenticeships (OJT, awareness training, formal/uniform use of this tool)Enhanced NDI procedures – deployment, signal interpretation, clearer schematics showing structural configurationUse of inspection coverage aids should be requiredDivide large area inspections into a number of smaller regionsAdd audible alarms & detection lights to probe in “Go”/”No-Go” devicesPrepare additional industry guidance to address training, use of NDI Reference and Proficiency specimens, procedures, composite construction awareness – produced by joint effort of OEMs, Airlines, FAA & industry groups
33 FAA Airworthiness Assurance Center Sandia National Laboratories 2013 Airlines for America NDT ForumPOD Studies to Quantify Flaw Detection in Composite Laminate StructuresDennis RoachTom RiceFAA Airworthiness Assurance CenterSandia National LaboratoriesComposites have many advantages for use as aircraft structural materials including their high specific strength and stiffness, resistance to damage by fatigue loading and resistance to corrosion. The aircraft industry continues to increase its use of composite materials, most noteworthy in the arena of principle structural elements. This expanded use, coupled with difficulties associated with damage tolerance analysis of composites, has placed greater emphasis on the application of accurate nondestructive inspection (NDI) methods. Traditionally, a few ultrasonic-based inspection methods have been used to inspect solid laminate structures. Recent developments in more advanced NDI techniques have produced a number of new inspection options. Many of these methods can be categorized as wide area techniques that produce two-dimensional flaw maps of the structure. An experiment was developed to assess the ability of both conventional and advanced NDI techniques to detect voids, disbonds, delaminations, and impact damage in adhesively bonded composite aircraft structures. A series of solid laminate, carbon composite specimens with statistically relevant flaw profiles were inspected using conventional, hand-held pulse echo UT and resonance, as well as, new NDI methods that have recently been introduced to improve sensitivity and repeatability of inspections. The primary factors affecting flaw detection in laminates were included in this study: material type, flaw profiles, presence of complex geometries like taper and substructure elements, presence of fasteners, secondarily bonded joints, and environmental conditions. This experiment utilized airline personnel to study Probability of Detection (POD) in the field and to formulate improvements to existing inspection techniques. In addition, advanced NDI methods for laminate inspections – such as thermography, shearography, scanning pulse-echo UT, ultrasonic spectroscopy, laminography, microwave and phased array UT – were applied to quantify the improvements achievable through the use of more sophisticated NDI. This paper presents the experiment design used to evaluate applicable inspection techniques and the key results from the POD testing conducted at multiple airline facilities.